structure of orthorhombic nbpo5
Post on 21-Sep-2016
Embed Size (px)
I. ABRAHAMS, M. C. PIENKOWSKI, P. G. BRUCE AND P. P. EDWARDS 733
In the final refinement there were no correlations between structural parameters above 35%. Refined atomic parameters are given in Table 1 with selected interatomic contact distances and angles in Table 2. The final difference profile is shown in Fig. 1" with views of the structure shown in Fig. 2.
Related literature. The structure determination of stoichiometric KCuO2 has been reported previously (Hestermann & Hoppe, 1969; Brese, O'Keeffe, von Dreele & Young, 1989). Electrical and magnetic data for the title compound are presented elsewhere (Pien- kowski et al., 1992).
* A list of primary diffraction data, i.e. the numerical intensity of each measured point on the profile as a function of scattering angle, has been deposited with the British Library Document Supply Centre as Supplementary Publication No. SUP 54711 (14 pp.). Copies may be obtained through The Technical Editor, International Union of Crystallography, 5 Abbey Square, Chester CHl 2HU, England. [CIF reference: HA0076]
We wish to thank the SERC for financial support and Dr P. Lightfoot for data collection. PGB grate- fully acknowledges the Royal Society for a Pickering Research Fellowship.
References BENDALL, P. J., FITCH, A. N. & FENDER, B. E. F. (1983). J. Appl.
Cryst. 16, 164-170. BRESE, N. E., O'KEEFEE, M., VON DREELE, R. B. & YOUNG, V. G.
JR (1989). J. Solid State Chem. 83, 1-7. DAVID, W. I. F., JOHNSON, M. W., KNOWLES, K. J., MORETON-
SMITH, C. M., CROSBIE, G. D., CAMPBELL, E. P., GRAHAM, S. P. 8g, LYALL, J. S. (1986). GENIE. A Language for Spectrum Manipulation and Display. Rutherford-Appleton Laboratory, Oxon OXll 0QX, England.
HAMILTON, W. C. (1965). Acta Cryst. 18, 502-510. HESTERMANN, K. & HOPPE, R. (1969). Z. Anorg. Allg. Chem. 367,
249-260. MOTrmRWELL, W. D. S. (1979). PLUTO. Program for plotting
molecular and crystal structures. Univ. of Cambridge, England. PIENKOWSKI, M. C., BRUCE, P. G., ABRAHAMS, I., JANES, R. &
EDWARDS, P. P. (1992), J. Mater. Chem. Submitted.
Acta Cryst. (1992). C48, 733-735
Structure of Orthorhombic NbPOs
Be DEBORAH L. SERRA AND SHIOU-Jw-I Hwu*
Department of Chemistry, Rice University, PO Box 1892, Houston, TX 77251, USA
(Received 17 June 1991; accepted 24 September 1991)
Abstract. Niobium phosphate, Mr = 203.88, ortho- rhombic, Pnma, a = 11.304(2), b--5.316(2), c = 6.640 (2) A, V= 399.0 (3) A 3, Z = 4, Dx = 3.39 g cm -3, A(Mo Ka) = 0.71069 A, p, = 31.8 cm-1, F(000) -- 384, T = 296 K, R = 0.030, wR -- 0.043 for 462 unique reflections (Rint=0.017) with Fo2> 3~r(Fo2). The framework is built up from NbO6 octa- hedra and PO4 tetrahedra. The NbO6 octahedra share opposite corners to form infinite zigzag chains along the b axis. These parallel octahedral chains are interconnected to each other via corner-sharing PO4 tetrahedra.
Experimental. Gem-shaped crystals of NbPO5 were obtained from a reaction in the K -Nb-P -O system. The single crystals were grown at 1375 K from a reaction with the target composition KNblzP6033. A crystal, with average dimensions 0.15 x 0.1 x 0.05 mm, was selected for indexing and intensity data collection. Diffraction data were collected by an to
* To whom all correspondence should be addressed.
scan (4o) min- 1, +__ 0.45 in to) at room temperature on a Rigaku AFC5S four-circle diffractometer equipped with a graphite monochromator. The unit- cell parameters and the orientation matrix for data collection were determined by the least-squares fit of 25 peak maxima with 7 < 20 < 27 . There was no detectable decay during the data collection according to the intensities of three standard reflections (1 21, 11 1, 33 1) measured every 100 reflections. Total of 1043 reflections (0_
734 ORTHORHOMBIC NbPO5
applied to the intensity data. The atomic coordinates were found using the direct Patterson method and are listed in Table 1.t A correction for secondary extinction was applied [9(1) 10-7]; IF~I = g-llF~l[x * +(1 + x'2)1/2] 1/2, x* is the value of x corresponding to a replacement of IF~I by K-11F~l (Zachariasen, 1968). The structure and thermal parameters were then refined by full-matrix least- squares methods based on F 2 of a unique data set to R = 0.030, wR = 0.043 and S = 1.90 for 41 variables, W = [or2(Fo)] -1, (d/o')max = 0.02. The maximum and minimum residual electron densities in the final difference Fourier map were 1.45 and -2.63 e A -3 respectively. Scattering factors from Cromer & Waber (1974).
The title compound NbPO5 crystallizes in the orthorhombic crystal system and axial photographs of the single crystal showed no sign of a superlattice. A projection onto the ab plane of the structure of NbPO5 is shown in Fig. 1. The structure is built up of NbO6 octahedra and PO4 tetrahedra. The four oxygen atoms, 0(2), 2 x 0(3), 0(4), of a PO4 tetra- hedron comer share with four NbO6 octahedra. The remaining two oxygen atoms, 2 x O(1), are oxo oxygens, and are available for Nb---O---Nb bonding between neighboring NbO6 octahedra. A resultant zigzag chain of NbO6 octahedra can be observed running along the b axis. The parallel corner-sharing NbO6 octahedral chains are interconnected through the PO4 tetrahedra to form a three-dimensional framework with an Nb:P ratio of 1:1.
Related literature. The orthorhombic cell of NbPO5 was first indexed by Levin & Roth (1970) using powder X-ray diffraction methods. The present study reports the single-crystal structure and details of the bond distances for orthorhombic NbPOs. A monoclinic cell for NbPO5 was first proposed by Chahboun, Groult, Hervieu & Raveau (1986) using electron diffraction. A single-crystal structure analy- sis by LeClaire, Chahboun, Groult & Raveau (1986) confirmed the monoclinic cell based on the space group P21/c (No. 14). The structure reported here and the monoclinic form are very similar. These two unit cells are related to each other by the following transformation matrix (o = orthorhombic, m = monoclinic): lol) (ao) (am)
010 bo = am 002 Co am
t Lists of structure factors and anisotropic thermal parameters have been deposited with the British Library Document Supply Centre as Supplementary Publication No. SUP 54610 (7 pp.). Copies may be obtained through The Technical Editor, Interna- tional Union of Crystallography, 5 Abbey Square, Chester CH1 2HU, England. [CIF reference: ST0536]
Table 1. Positional and isotropic thermal parameters for NbPO5
Anisotropically refined atoms are given in the form of the iso- tropic equivalent displacement parameters defined as B~q = (8~-2/3) trace U.
Wyckoff notation x y z B~q(A 2)
Nb 4(c) 0.43757 (5) ~ 0.33111 (9) 0.58 (3) P 4(c) 0.1544 (2) 0.5282 (2) 0.59 (6) O(1) 4(a) 0 0 0 2.5 (3) 0(2) 4(c) 0.0818 (5) ~ 0.3353 (8) 1.7 (2) 0(3) 8(d) 0.1287 (4) 0.018 (1) 0.6477 (7) 3.9 (2) 0(4) 4(c) 0.2852 (4) :I 0.4719 (8) 1.1 (2)
Table 2. Selected bond distances (A) for NbO 6 and PO 4/n NbPO5
NbO6 octahedron PO4 tetrahedron Nb--O(l i'ii) 1.8764 (4) (2 x ) P--O(2) 1.519 (4) Nb-43(2 i) 1.973 (4) P--O(3 ~) 1.499 (3) (2 x ) Yb---O(3 ill'iv) 2.015 (3) (2 x ) P--O(4) 1.523 (4) Nb--O(4) 1.959 (4)
1 l (il) x_ : Symmetry codes: (i) + x, ~ - y, ~ - z; , - + z; (iii) -x , -y , z -; ( iv ) -x , +y,z - - ; t ) , - -Y , y '
Fig. 1. Projection onto the ab plane of the structure of ortho- rhombic NbPO5.
The bond distances (Table 2) are comparable to those observed in the monoclinic cell except for the P--O(3) bonds which are significantly shorter.
Acknowledgement is made to the donors of the Petroleum Research Fund, administered by the ACS (grant ACS-PRF21154-63), and the National Science Foundation, Solid State Chemistry (SGER) (grant DMR-9012983), for support of this research. DLS is indebted to the Dow Chemical Co. for a fellowship (1990-1991). Financial support for the single-crystal X-ray diffractometer by the National Science Foundation is gratefully acknowledged.
References Cnansotn~, H., GROULT, D., HERVmU, M. & R.hV~U, B. (1986).
J. Sol id State Chem. 65, 331-342.
DEBORAH L. SERRA AND SHIOU-JYH HWU 735
CROMER, D. T. & WABER, J. T. (1974). International Tables for X-ray Crystallography, Vol. IV, pp. 71, 148. Birmingham: Kynoch Press. (Present distributor Kluwer Academic Publishers, Dordrecht.)
LECLAIRE, A., CHAHBOUN, H., GROULT, D. & RAVEAU, B. (1986). Z. Kristallogr. 177 (3-4), 277-286.
LEWN, E. & Roan, R. (1970). J. Solid State Chem. 2, 250- 261.
Molecular Structure Corporation (1989). TEXSAN. TEXRAY Structure Analysis Package. Version 5.0. MSC, 3200A Research Forest Drive, The Woodlands, TX 77381, USA.
ZACHARIASEN, W. H. (1968). Acta Cryst. A24, 212-216.
Acta Cryst. (1992). C48, 735-737
Structure of an Iridium Bis(phosphine)diene Complex, a Catalyst for Homogeneous Hydrogenation
BY P. A. CaALONER, P. B. HIT.CHCOCK AND M. REISINGER
School of Chemistry and Molecular Sciences, University of Sussex, Falmer, Brighton, England
(Received 15 July 1991; accepted 3 September 1991 )
Abstract. (,/74_ 1,5-Cyclooctadiene)bis(triphenylphos- phine)iridium(I) hexafluorophosphate, [Ir(C8H~2)- (PPh3)2][PF6], C44H42F6IrP3.0.5CH2C12, Mr = 1012.4, monoclinic, P21/c, a=11.666(1), b=18.885(3), c=19.492(2) A, f l=97.07(1) , V=4261.7A 3, Z=4, Dx=1.58 gcm -3, A(MoKa)=0.71069~, /z=33.5cm-~, F(000)=2012, T=295K, R= 0.050, wR=0.070 for 5438 observed reflections with IF21 >2or(F2). The geometry at iridium is approximately square planar, but the iridium--phos- phorus bond lengths are significantly different: Ir--P1 2.367 (2), Ir--P2 2.326 (3)/~, P I - - I r - -P2 = 94.3 (1), MI -